Borates <i>vs</i>. aluminates: comparing the anion for lithium-ion batteries.
Ould, Darren M. C.; Penrod, Megan E.; McConnell, Jessica B.; Zabara, Mohammed A.; Berge, Astrid H.; O'Keefe, Christopher A; Bond, Andrew D.; Menkin, Svetlana; Grey, Clare P.; Wright, Dominic S.; Chemical communications (Cambridge, England) 61 (2024) 129–132; doi:10.1039/d4cc04812a

data_7133996
_publ_section_title
;
 Borates <i>vs</i>. aluminates: comparing the anion for lithium-ion
 batteries.
;
_journal_issue                   1
_journal_name_full               'Chemical communications (Cambridge, England)'
_journal_page_first              129
_journal_page_last               132
_journal_paper_doi               10.1039/d4cc04812a
_journal_volume                  61
_journal_year                    2024
_chemical_formula_moiety         'C16 H14 Al F24 Li O6'
_chemical_formula_sum            'C16 H14 Al F24 Li O6'
_chemical_formula_weight         792.19
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2019/2
_audit_update_record
;
2024-06-04 deposited with the CCDC.	2024-11-22 downloaded from the CCDC.
;
_cell_angle_alpha                78.701(3)
_cell_angle_beta                 73.361(3)
_cell_angle_gamma                79.766(3)
_cell_formula_units_Z            2
_cell_length_a                   10.1045(6)
_cell_length_b                   10.3479(6)
_cell_length_c                   15.5279(9)
_cell_measurement_reflns_used    5934
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      67.95
_cell_measurement_theta_min      3.01
_cell_volume                     1512.65(16)
_computing_cell_refinement       'SAINT (Bruker, 2016)'
_computing_data_collection       'APEX5 (Bruker, 2023)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'Mercury (Macrae et al., 2008)'
_computing_publication_material  SHELXL
_computing_structure_refinement  'SHELXL (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'Bruker D8-QUEST PHOTON-III'
_diffrn_measurement_method       '\w and \f-scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0589
_diffrn_reflns_av_unetI/netI     0.0444
_diffrn_reflns_Laue_measured_fraction_full 0.990
_diffrn_reflns_Laue_measured_fraction_max 0.987
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            22760
_diffrn_reflns_point_group_measured_fraction_full 0.990
_diffrn_reflns_point_group_measured_fraction_max 0.987
_diffrn_reflns_theta_full        67.679
_diffrn_reflns_theta_max         68.368
_diffrn_reflns_theta_min         3.006
_diffrn_source                   'Incoatec I\mS Cu microsource'
_exptl_absorpt_coefficient_mu    2.307
_exptl_absorpt_correction_T_max  0.7531
_exptl_absorpt_correction_T_min  0.6440
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Bruker, 2016)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.739
_exptl_crystal_description       block
_exptl_crystal_F_000             780
_exptl_crystal_size_max          0.160
_exptl_crystal_size_mid          0.160
_exptl_crystal_size_min          0.160
_refine_diff_density_max         0.565
_refine_diff_density_min         -0.437
_refine_diff_density_rms         0.082
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.079
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     435
_refine_ls_number_reflns         5486
_refine_ls_number_restraints     144
_refine_ls_restrained_S_all      1.174
_refine_ls_R_factor_all          0.1003
_refine_ls_R_factor_gt           0.0819
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1395P)^2^+0.9813P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2282
_refine_ls_wR_factor_ref         0.2494
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4090
_reflns_number_total             5486
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d4cc04812a2.cif
_cod_data_source_block           DW_B1_0553
_cod_depositor_comments
'Adding full bibliography for 7133996--7133998.cif.'
_cod_database_code               7133996
_cambridge_user_name             'Darren Ould'
_cambridge_user_crsid            dmo33
_cambridge_supervisor_name       'Dominic Wright'
_cambridge_supervisor_crsid      dsw1000
_cambridge_crystallographer_name 'Andrew Bond'
_cambridge_crystallographer_crsid adb29
_cambridge_sample_id             EXP306
_cambridge_data_id               DW_B1_0553
_shelx_estimated_absorpt_t_min   0.709
_shelx_estimated_absorpt_t_max   0.709
_shelx_res_checksum              71549
_shelx_hkl_checksum              30145